Tribology in Industrywww.tribology.rs
Wear Resistance Increase of Samples Tribomating
in Oil Composite with Geo Modifier КGМF-1
, O. Lyashukb
, A. Hrinkiva
, D. Velykodnyia
, Y. Vovkb
, D. Holuba
, A. Chernaia
aCentral Ukrainian National Technical University, 8 Universytetskyi ave., 25006 Kropyvnytskyi, Ukraine,
bTernopil Ivan Puluj National Technical University, 56 Ruska str., 46001 Ternopil, Ukraine.
Tribomating of sample Geo modifier
Composite oil Friction torque Wear resistance Acoustic emission Friction area Oil M-10G2K
Cuprum glycerate XADO
A B S T R A C T
Increase of wear resistance of different types of tribomating which are functioning in fluid lubrication is possible due to: choosing more expensive and high quality material of samples that is not always sensible; applying some wear resistant coatings on them; selection and formation of complex composition of oil additives. Due to nanomaterials development there is a possibility of efficient use of functional additives such as geo modifiers in tribology. Due to geo modifier-based oil composites use it’s not necessary to make any structural changes of machines mated parts though their wear resistance is increased. It requires the conducting of some experimental tribological research. It was found that oil media modified by a geo modifier increase the wear resistance of working surfaces of different types of tribomating. The use of geo modifier КGМF-1 (Katerynivka friction geo modifier -1 (patent of Ukraine №69657)) has been suggested. Lubrication quality of oil compositions based on М-10Г2К (M-10G2K) (motor oil of 10th
viscosity grade, of group Г2К (G2K), for the CIS countries the oil grade
conforms SAE 30) + КGМF-1 (4.0 - 4.5%) has been studied on a computer modernized four-ball friction testing machine ЧШМ-К1 (CHMK-К1). To evaluate the lubrication quality of the oil composite with the suggested geo modifier and to use the comparative analysis of the obtained results the research was conducted on commercial samples of base oil M-10G2K and oil
composites M-10G2K + XADO Maximum for Diesel Truck (2.0 - 2.3%) (agent
2D sliding revitalization factor (RF) 100, revitalizant 1 Stage RF 100, metal conditioner RF 5.5), M-10G2K + cuprum glycerate (3.7 - 4.5%). Some average
indices of wear, critical load, and welding load have been found. Samples division into 4 types of mating according to the following characteristic features: mobility, material hardness and friction area has been suggested for more accurate picture of wear resistance changes of samples tribomating which are functioning in base and modified oil. Lower friction torque of different samples couplings in modified oil by geo modifier КGМF-1 in comparison with base oil M-КGМF-10G2K was recorded while using Friction
machine 2070 SMT-1 with add-on module "ring-ring". The samples wear rate in modified oil by geo modifier КGМF-1 in comparison with base oil M-10G2K was studied by method of acoustic signal amplitude measurements
directly from the friction zone by a commercially produced instrument of Brüel & Kjear company.
Central Ukrainian National Technical University, 8 Universytetskyi ave., 25006 Kropyvnytskyi, Ukraine. E-mail: AulinVV@gmail.com
It was found that efficiency increase of the oil compositions under investigation is taking place in the following order: M-10G2K + XADO
Maximum for Diesel Truck, M-10G2K + cuprum glycerate, M-10G2K +
КGМF-1. Wear index due to the use of modified oil M-10G2K + КGМF-1 was
19 - 20 % lower comparing to the obtained data of the base oil, critical load value was 27 - 29 % larger, and welding load – 24 - 25% larger respectively. Moreover, it was recorded that the maximum wear rate of samples in their functioning in modified oil M-10G2K + КGМF-1 was 3
times lower, and friction torque change law is similar to the wear rate change depending on the time of testing.
© 2019 Published by Faculty of Engineering
One of the ways to increase the wear resistance of machine parts tribomating is their use with more functionally adaptable lubricants with different synthetic additives and geo modifiers. Nowadays the lubricating properties of oils are improved mainly due to commercial additive complexes. Oil additives based on natural minerals after their pretreatment are called geo modifiers. Some papers describing the effect of geo modifiers use admit that surface-active substances of a metal-ceramic reconditioner being used on friction areas with some oil provoke the process of formation of a highly wear resistant metal-ceramic coating with lower friction coefficient on the mated surfaces. Due to these additives in oil medium some friction surface texturing takes place with simultaneous hardening of the main material at great depth on the samples tribomating surfaces. While tribomating is taking place some rational micro relief is being created on the samples surfaces which are correspondent to the actual operating conditions. The most popular additives on the Ukrainian market are those represented by trade mark XADO which have shown good results for power-supply units of transport vehicles.
The distinctive feature of friction geo modifiers from other additives consists in adding some substances to the samples tribomating which launch the self-organization processes [1-4]. At the same time, mainly by adding some additives into oil, mated surfaces are being separated by soft metals  and long hydrocarbon chains, synthesized film. It contributes to the surface optimal structure developing, especially in the contact areas with maximum number of available bonds resulting in increased oil confinement ability and equilibrium roughness . Moreover,
the development of matters dealing with geo modifiers use in oil compositions enables us to increase the tribomating samples wear resistance and their further commercial use to obtain various positive effect under machines maintenance conditions.
2. LITERATURE REVIEW
characteristics and repairing compositions with additives of natural origin which are based on serpentinite-based powder properties have been studied in the papers [13-16]. The data of conducted investigation haven’t shown the real comparative picture of wear with existing synthetic additives. Although, the authors in
papers [13-16] gave some theoretical
substantiation of oil compositions use with some friction geo modifiers of this type in tribomating under investigation.
Geo modifiers stimulate mechanical and chemical reactions, oil components pyrolysis and tribo catalytic carbonization, graphitization and creation of hard carbon containing oil compounds [16,17]. The conditions of coatings formation, low friction and heat conductivity coefficient, high hardness and corrosion resistance of geo modifiers have been found. These conclusions can be made due to the study of geo modifiers Mg6Si4O10(OH)8 properties . It was found that
friction geo modifiers were based on a large group of minerals with similar chemical formula where Mg can be replaced by iron and nickel [2,13,16]. Serpentinite rock includes several types of serpentinite, magnetite and chromium and various chemical elements used as geo modified composition mixture [10,14]. The study of various geo modified compositions have been highlighted in papers [5,6,10,19], some recommendations have been given dealing with their efficient use in wear-reversing tribo technologies development [15-16].
Chemical constituent of metal-ceramic layer formation from geo modifiers has been developed to a certain extent in the paper , but there is no information on physical-mechanical and rheological properties of these layers. There is no practical evidence. Some published papers assume the possibility of occurring an elastic-hydro-dynamic effect characterized by high pressure in an oil-film wedge causing the elastic deformation of samples materials which are in contact. Due to this a gap size between parts is getting bigger. Apparently, this happens while a layer is being formed when geo modifiers are in the oil [17,21,22]. Deep investigation of surface and pre-surface layers formed on the friction surfaces under treatment by geo modifiers conditions haven’t been found in open sources.
There has been no study of wear resistance increase dynamics of oil compositions with some friction geo modifiers so far. Wear resistant coatings, definitely, have dissipative and metastable structures . Tribotechnical oil compositions with some geo modifiers aren’t systematized and need some further research of their efficiency for tribomating concerning wear resistance increase.
The purpose of the paper is to increase the wear resistance of samples couplings in oil medium with Katerynivka friction geo modifier-1 (КGМF-1) and to make the comparative analysis according to tribotechnical characteristics of base oil and oil composites with adding the commercial sample of XADO  Maximum for Diesel Truck additive and cuprum glycerate respectively. The purpose has been achieved by solving the problems:
study on the 4-ball friction machine
ЧШМ-К1 (CHMK-ЧШМ-К1) the wear index, critical load, welding load for the base oil М-10Г2К
(M-10G2K), oil compositions motor oil of 10th
viscosity grade, of group Г2К (G2K), for the
CIS countries the oil grade conforms SAE
30), M-10G2K + cuprum glycerate, M-10G2K +
XADO Maximum for Diesel Truck, M-10G2K +
according to the obtained results analyze
the lubrication capability of oil composite with geo modifier КGМF-1 and compare it
with the efficient oil composites M-10G2K, +
cuprum glycerate, M-10G2K + XADO
Maximum for Diesel Truck,
find the laws of friction torque change and
wear rate of different types of samples mating due to the use of oil composition
M-10G2K + КGМF-1 according to the the
scheme “ring-ring” on the friction machine 2070 SMT-1.
3. MATERIALS AND METHODS
lorries which are widely represented in central regions of Ukraine and hydraulic units .
Motor oil M-10G2K (base oil) widely used for
KamAZ-family lorries maintenance and oil composites: M-10G2K + КGМF-1 (4.0 - 4.5) were
used as a lubricating environment. The preliminary results of КGМF-1 content were
described in the paper , M-10G2K + cuprum
glycerate (3.7 - 4.5%) - in the paper . For the
comparative study the oil composition M-10G2K +
XADO Maximum for Diesel Truck (made in Ukraine), (2.0 - 2.3%) concentration was according to the manufacturer’s requirements. We must admit that geo modifier КGМF-1 mixture was obtained from clay-based natural substances, it’s main physical properties were recorded and described by the group of authors of Central Ukrainian national technical university in the patent of Ukraine № 69657 .
Due to the point contact of the samples four-ball wear test system ЧШМ-К1 is quite a reliable instrument for determining the lubrication capability of base oils and their composites, lubricants additives efficiency. The study of wear-reversing mixture КГМТ-1 (KGMF-1) use efficiency in base oil M-10G2K has been carried
out on ball samples by point or line contacts. As comparative study some tests on base oil
M-10G2K and oil composition M-10G2K + XADO have
been done. Tribomating process itself took place in four-ball wear test system CHMK-К1 where oil environment was tested. In fact, the mating itself took place in a pyramid of 4 balls where three lower balls were fixed solid in a cup filled with tested oil and the upper ball was rotating in a vertical spindle. Four-ball wear test system CHMK-К1 was used in investigating the lubrication capability of base and composite lubricants . The average values of critical load, welding load and wear index characterized by a wear scar diameter-applied load ratio for certain oil media were measured in the investigation. The use of four-ball wear test system CHMK-K1 is specified by GOST 9490-75, in Germany – by DIN 51350, and in the USA – by ASTM D2783 .
Friction machine 2070 SMT-1 (a) with add-on module of "ring-ring" type (Fig. 1) has been used for the study of laws of friction torque change and wear rate of samples mating to find their wear resistance increase and prove the efficiency of oil
composites use with geo modifier КGМF-1. Base and composite oils were supplied to the friction zone by a gear pump through a nozzle. A fine filter till particles of 10 mcm size was installed in lubrication system to avoid wear particles impact on friction and wear parameters.
Fig. 1. (a) Friction machine 2070 SМТ-1, (b) with add-on module "ring-ring".
An add-on module was mounted to implement the model. General view of the samples is given by Fig. 2.
Fig. 2. (а) Experimental models for "ring-ring" tester on friction machine 2070 SMT-1: Бр. АЖ 9-4 (CuA19Fe3) (НВ95), and (b) СЧ 18 (equivalent EN-GJL-200) (HRC40).
Before the investigation the samples had been wearing in till the complete contact areas took place. Here, the surface roughness was equal
to Ra0.2 mcm that corresponds to wear-in
mating of resources defining mating of power units of transport and hydraulic machines. The
roughness measurements were made
according to GOST 27964-88 using a profilometer (roughness indicator) of make 283. The investigation was conducted with the
coefficient of mutual overlap Kb30.5, caused
by involving more types of samples mating. The samples size and testing procedure were specified by GOST 23.210.
samples according to GOST Р 51860-2002 of friction machine 2070 SMT-1. The samples of "ring-ring" type have the outer diameter 12 mm, and inner diameter 6 mm.
To have more accurate picture of changes of mated samples wear resistance due to their functioning in base and modified oil their division according to the samples features has been suggested. For the friction machine 2070 SMT-1 the mating is divided into 4 types according to the characteristic features: mobility, material hardness, friction zone area (Table 1).
Table 1. Types of tribomated samples (parts) and characteristic features.
Characteristic features of tribomated samples (parts)
Type of mating
Movable sample (part) Stationary sample (part) Material
hardness, Нр Friction area, Sр hardness, Material
Friction area, Sн
І Нm> Нf Sm> Sf Нf < Нm Sf < Sm ІІ Нm < Нf Sm> Sf Нf > Нm Sf < Sm ІІІ Нm> Нf Sm< Sf Нf < Нm Sf > Sm ІV Нm < Нf Sm< Sf Нf > Нm Sf > Sm
The first type of tribomated samples is widely used where the material of a movable sample (part) is harder (Нр) and friction zone area (Sр) is
larger, whereas a stationary sample is less hard (Нн) and its friction zone area (Sн) is smaller.
Нр<Нн, Sр>Sн is a characteristic feature of the
second type of tribomating, Нр>Нн, Sр<Sн is for the
third type, and Нр<Нн, Sр<Sн is for the fourth one.
Wear rate of hard and soft materials of mated samples (parts) of the fourth type is the same.
The first type of tribomating is mating of a steel shaft and a soft bushing that is widely used in systems and units of mobile agricultural and motor transport vehicles and are quite popular due to their performance characteristics. Tribomating of hard chrome-plated cylindrical samples and a soft steel movable disc belong to the second type. Hydro cylinder and its mated steel piston (here the cylinder is made of softer steel) represent the third type of mating. Tribomating “cylinder liner-piston” is of the fourth type.
During the investigation the friction torque change was found by the friction force and a sample size, and wear rate – by the acoustic signal amplitude from friction zone.
The processes of tribomated parts and samples wear were studied by method of acoustic emission . An acoustic-emission complex was used in the investigation. It consisted of a commercially produced instrument of Brüel & Kjear company (type 2511).
Fig. 3. A set for wear rate study by measuring the acoustic signal amplitude.
A piezoelectric element made by Brüel & Kjear company fixed on the stationary sample was used as a transducer. The complex allows for transducing the acoustic signals of tribomated samples under the tests conditions. The choice of acoustic emission parameters is very
important in conducting tribological
investigation as it reflects adequately the wear processes taking into account the specific features of the signal formation. An amplitude signal from the friction zone area correlated with the wear rate value was chosen as an information characteristics of acoustic emission to study the dynamics of the wear resistant layer formation and damage. A calibrated diagram was built to transform the values of signal acoustic emission amplitude from the friction zone into wear rate values.
To convert the values of acoustic emission amplitude of the signal formed in the friction zone into the wear rate values the following formula was used:
I k A (1)
where k = 0.4 mV-1 – a conversion factor found
by the calibrated diagram for the device of Brüel
& Kjear company (type 2511); А – acoustic
signal amplitude, mV.
The device of Brüel & Kjear company (type 2511) conditioning was done by means of acoustic signal frequency selection which showed the wearing processes of the tribocoupling samples under study the most
adequately. The conditioning under
any contacts of the samples and the obtained results of acoustic signals amplitude were neglected as noises. The values of their amplitudes were set at threshold quantity, so in wear rate estimating by means of the device of Brüel & Kjear company (type 2511) they were neglected. The rational frequency of the samples’ wear rate estimation due to the surface layers formation and failure in base and modified oil media with the samples under consideration being in contact was equal to 4 kHz. This value corresponds to the maximum amplitude of acoustic signal within range of frequency 3…6 kHz of acoustic spectrum neglecting the noises. The above-mentioned frequency of acoustic signals corresponds to the most accurate and adequate results of wear rate evaluation of the samples under consideration by acoustic emission comparing to the gravimetric method.
Experimental research of different types of samples mating was conducted to obtain the values of wear rate Iu and friction torque Мfr in
base M-10G2K and composite M-10G2K+КGМF-1
oils. The overall time of the experiment was 100 - 110 min. In each case a diagram of acoustic emission amplitude and friction torque changes was recorded by a self-recording device.
Oil composite M-10G2K with geo modifier КGМF-1
was compared with base oil М-10Г2К and oil
compositions M-10G2K + cuprum glycerate,
M-10G2K + ХАDО Maximum for Diesel Truck.
Lubrication capability of the oil samples under consideration was testing on CHMK-К1 by the following indices: wear, critical load and welding load. The results of the study are given in the Table 2.
Table 2. Average results of tests on the four-ball wear test system CHMK-К1 in different lubrication media.
ХАDО M-10GКGМF-1 2K + Wear
mm 0.56±0.03 0.48±0.02 0.52±0.03 0.45±0.02 Critical
load, N 1236±1.0 1520±2.0 1490±2.0 1570±3.0 Welding
load, N 1962±15.0 2420±25.0 2350±10.0 2452±10.0
According to results of investigation on the four-ball wear test system CHMK-К1 the low layers wear scar of average diameter-vs-applied load curves were plotted. Time period per test according to GOST 9490-75 is equal to 10 sec.
Fig. 4. Wear scars average diameter-vs-applied load curves for different lubricants: 1 – motor oil M-10G2K (base lubricant); 2 – M-10G2K + cuprum glycerate; 3 – M-10G2K + ХАDО Maximum for Diesel Truck; 4 – M-10G2K + КGМF-1.
The results of studying the evolution of friction torque change on friction machine 2070 SMT-1 (Table 3) and wear rate (Table 4) are shown for
different tribocoupling types in base oil M-10G2K
and oil with geo modifier КGМF-1. Steel 45 and СЧ 18 (equivalent EN-GJL-200) (analogEN-GJL-200) were used as materials of samples mating.
The results of study of regularities of friction torque change and wear rate change of the I - IV types of samples tribomating from steel 45 - Бр.Аж 9-4 (CuA19Fe3) are given on Figs. 5-8 respectively.
Table 3. Regularities of friction torque change Мfr (10
-3N·m) in different types of samples mating in base oil M-10G2K (A) and composite M-10G2K + КGМF-1 (В) depending on time of testing (steel 45 and СЧ 18 (equivalent EN-GJL-200) as samples materials).
Type of mating Oil
Time of test, min.
0 10 20 30 40 50 60 70 80 90 100
B ±0.07 1.2± ±0.13 2.7± ±0.14 2.8± ±0.12 2.7± ±0.09 2.2± ±0.09 2.0± ±0.10 2.0± ±0.11 1.9± ±0.07 1.8± 1.8± ±0.1 ±0.09 1.7±
B ±0.07 1.7± ±0.09 2.2± ±0.13 3.0± ±0.14 2.9± ±0.13 2.8± ±0.12 2.9± ±0.11 2.9± ±0.11 2.9± ±0.12 2.9± ±0.09 2.9± ±0.15 2.9±
±0.01 ±0.13 2.5± ±0.10 2.4± ±0.12 2.3± ±0.13 2.3± ±0.12 2.3± ±0.11 2.3± ±0.13 2.3± 2.3± ±0.1 ±0.09 2.3± ±0.12 2.3±
B ±0.02 1.0± ±0.11 2.1± ±0.08 1.9± ±0.07 1.9± ±0.08 1.8± ±0.07 1.8± 1.8± ±0.1 ±0.08 1.8± ±0.09 1.8± ±0.11 1.8± ±0.08 1.8±
±0.12 ±0.18 4.1± 4.2± ±0.2 ±0.19 4.2± ±0.21 4.0± ±0.14 3.7± ±0.16 3.6± ±0.14 3.6± ±0.12 3.5± ±0.16 3.7± ±0.15 3.7±
Тable 4. Regularities of wear rate change Iu (10–9) in different types of samples mating in base oil M-10G2K (A) and oil composite M-10G2K + КGМF-1 (В) depending on the time of testing (Steel 45 - СЧ 18 (equivalent EN-GJL-200) as samples material).
mating Oil 0 10 20 30 40 50 60 70 80 90 100 Time of test, min.
±0,01 0,55± ±0,01 0,59± ±0,03 0,58± ±0,25 0,57± ±0,04 ±0,04 0,57± 0,58± ±0,03 0,57± ±0,02 0,57± ±0,01 0,57± ±0,02 0,57± ±0,03
B 0,28± ±0,03 ±0,02 0,4± 0,39± ±0,04 0,38± ±0,18 0,30± ±0,01 0,24± ±0,02 0,22± ±0,01 0,21± ±0,01 ±0,01 0,2± ±0,02 0,2± ±0,01 0,2±
B ±0,01 0,2± 0,45± ±0,02 0,45± ±0,02 0,45± ±0,03 ±0,03 0,5± 0,55± ±0,02 0,55± ±0,02 0,57± ±0,03 0,58± ±0,01 ±0,01 0,6± ±0,02 0,6±
B ±0,03 0,5± 0,65± ±0,03 ±0,01 0,2± ±0,01 0,2± ±0,01 0,2± ±0,01 0,2± ±0,01 0,2± 0,29± ±0,02 ±0,01 0,2± ±0,03 0,2± ±0,01 0,2±
±0,01 0,64± ±0,03 ±0,01 1,0± 1,21± ±0,06 1,38± ±0,06 ±0,05 1,43± 1,54± ±0,08 1,58± ±0,04 1,59± ±0,03 ±0,05 1,6± ±0,02 1,6±
B ±0,02 0,4± ±0,02 0,6± ±0,05 1,2± 1,15± ±0,02 ±0,18 3,6± 1,22± ±0,03 1,21± ±0,05 1,21± ±0,04 ±0,02 1,2± ±0,03 1,2± ±0,05 1,2±
Fig. 5. (а) Evolution of friction torque in time, and (b) wear rate of the tribocoupling samples of the 1st type in time: 1 – base oil М-10G2К; 2 – base oil М-10G2К + КGМF-1.
Fig. 6. (а) Regularities of friction torque change, and (b) wear rate change of tribocoupling samples of the 2nd type, in time, with different lubricants: 1 – base oil М-10G2К; 2 – base oil M-10G2K + КGМF-1.
Fig. 7. (а) Regularities of friction torque change, and (b) wear rate of tribocoupling samples of the 3rd type with runtime: 1 – base oil М-10G2К; 2 – base oil М-10G2К + КGМF-1.
Fig. 8. (а) Regularities of friction torque change, and (b) wear rate of tribocoupling samples of the 4th type in time: 1 – base oil М-10G2К; 2 – base oil М-10G2К + КGМF-1.
According to the obtained results of tests on the four-ball wear test system CHMK-К1 (Table 1) the lubrication capability of oil composites
М-10G2К + cuprum glycerate, M-10G2K + ХАDО
Maximum for Diesel Truck, M-10G2K + КGМF-1
has been improved comparing to the base oil: the wear indes became lower, critical load and welding load values got increased. Oil composite with geo modifier КGМF-1 has proved to obtain the best results comparing to the base oil: wear index became 19 - 20 % lower, though critical load became 27 - 29 % larger. Scuff-resistance characteristics determined by welding load were 24 – 25 % improved. It can be explained by the fact that geo modifier КGМF-1 helps to improve the lubrication capability of oil composite as its particles in oil on the ball samples surfaces in friction zone act as additional lubricants.
Positive properties of oil composites M-10G2K +
cuprum glycerate, M-10G2K + ХАDО Maximum for
Diesel Truck, M-10G2K + КGМF-1 comparing to
the base oil M-10G2K can be observed on Fig. 4.
This is proved by low balls wear scar diameter-vs-applied load curves on CHMK-К1. It was found that most of additives such as cuprum glycerate – curve 2, ХАDО Maximum for Diesel Truck – curve 3, КGМF-1 – curve 4 make the welding load Pw
higher. Thus, while being added into base oil the above-mentioned additives will improve the scuff-resistance characteristics of base oil.
Moreover, all above-mentioned additives
increase the critical load value Pc characterizing
the anti-wear additives operation range. In general, the proposed additive KGMT-1 is similar to the blend XADO Maximum for Diesel Truck and
cuprum glycerate by scuff-resistance
characteristics but it provides more efficient performance of the oil composite.
The study has proved that the efficiency increase of lubrication capability of lubrication media of base and composite oils can be presented in the
following ordered series: M-10G2K, M-10G2K +
ХАDО Maximum for Diesel Truck, M-10G2K +
cuprum glycerate, M-10G2K + КGМF-1. Having
compared the obtained results, we came to the conclusion that further study of tribotechnical characteristics will be effective on base and
composite M-10G2K + КGМF-1 oils.
When an additive КGМF-1 is used in base oil M-10G2K on samples mating of material steel 45 -
СЧ18 (equivalent EN-GJL-200) the friction torque is getting 5 – 28 % decreased comparing to the base oil (Table 3) for different types of samples mating. In this case, it was found that wear rate (Table 4) is getting smaller on different types of samples mating in a different way: 1.5 - 2.5 times smaller for the I type of mating; 1.3 - 2.1 times smaller for the II type of mating; 4.2 - 5.7 times smaller for the III type of mating; 1.2 - 1.3 times smaller for the IV type of mating.
Wear rate is changing while operating in oil composite with geo modifier КGМF-1 adding. It was found that friction torque in different types of samples mating of material steel 45 – Бр.АЖ 9-4 (CuA19Fe3) had 15 - 33% smaller values comparing to the base oil (Figs. 5а - 8а). We came to the conclusion that composite oil with КGМF-1 use made wear rate 3.0 - 3.4 times lower for the I type of mating (Fig. 5b); 1.5 - 1.6 times lower for the II type of mating (Fig. 6, b) and IV type (Fig. 8b) respectively; 5.0 - 6.0 times lower for the III type of mating (Fig. 7b).
This wear process behavior can be explained by the fact that the particles of КGМF-1 are charging into soft surface of the samples. After charging is over the friction torque value is getting smaller. The further behavior corresponds to the friction torque change respective to the base oil but with a smaller value. In this case, wear rates of samples mating in base oil and composite oil with КGМF-1 are completely different.
may assume that the further development of additives formation technologies on its basis is a promising direction for heavily loaded mated parts maintenance.
1. The study of lubrication capability of base and
composite oils M-10G2K + cuprum glycerate,
M-10G2K + XADO Maximum for Diesel Truck,
M-10G2K + КGМF-1 has proved the positive
effect in comparison with base oil М-10G2К.
The improvement of such characteristics as welding load Pw, and critical load Pc, behavior
CHMK-K1 low balls wear scar diameter
respective to the applied load are the evidences. The composite oils under consideration can be used for tribomating wear resistance improvement.
2. It was found that among oil composites
under consideration M-10G2K + cuprum
glycerate, M-10G2K + ХАDО Maximum for
Diesel Truck, M-10G2K + КGМF-1 the oil
composite with geo modifier КGМF-1 has shown the best result comparing to the base oil: wear index became 19 - 20 % lower, though critical load became 27 - 29 % larger. Scuff-resistance characteristics determined by welding load were 24 - 25% improved.
3. Regularities of friction torque change and wear
rate of the samples respective to the time of testing on friction machine 2070 SMT-1 depend on their material, mating type and lubrication medium. Due to geo modifier КGМF-1 use in base oil M-10G2K on samples mating of the
material steel 45 - СЧ18 (equivalent EN-GJL-200) the friction torque is getting 5 - 28% smaller for different types of mating comparing to the base oil. Moreover, it was found that maximum decrease (4.2 - 5.7 times) of wear rate was obtained for the III type of mating, whereas minimum value (1.2 - 1.3 times) was obtained for the IV type of mating.
It was found that friction torque in different types of samples mating of material steel 45 – Бр. АЖ
9-4 (CuA19Fe3) in composite oil M-10G2K +
КGМF-1 medium had 15 – 33 % smaller values comparing to the base oil. The maximum wear rate decrease (5.0 - 6.0 times) was observed for the III type of samples mating, and the minimum
decrease (1.5 - 1.6 times) was observed for the II type of samples mating.
 V. Aulin, V. Slon, S. Lysenko, D. Holub, Research of Change of The Power of the Diesel of Cars Working in Non-Stationary Conditions, MOTROL. Commission of Motorization and Energetics in Agriculture, vol. 17, no. 2, pр. 103-108, 2015. [in Ukrainian]
 V. Aulin, V. Slon, S. Lysenko, The Character of Change of Tribo-Technical Descriptions of Interfaces of Diesels During Their Work in the Different Modes, The Problems of Tribology. Khmelnytskyi, no. 3, pр. 89-96, 2013. [in Ukrainian]
 V. Aulin, A. Hrinkiv, A. Dykha, M. Chernovol, O. Lyashuk, S. Lysenko, Substantiation of Diagnostic Parameters for Determining the Technical Condition of Transmission Assemblies in Trucks, Eastern European Journal of Enterprise Technologies, vol. 2, no. 1(92), pp. 4-13, 2018,
 А.P. Pavlov, N.G. Petrov, Comparative Analysis of Motor Oil Additives Characteristics Sold on Russian Market, Automobile. Road. Infrastructure, vol. 2, no. 12, pp. 5-12, 2017. [in Ukrainian]
 М.N. Svyryd, А.P. Kudryn, L.B. Pryimak, Use of ХАDО-additives in Tribomagnetic Reconditioning,
Bulletin of Khmelnytskyi National University, vol. 6, pp. 122-125, 2011. [in Ukrainian]
 D.А. Gomon, А.М. Dudka, І.І. Nachovnyi, Comparative Study of Motor Oil Anti-Wear Additives Performance. VIII International scientific-technical conference «Chemistry and Modern Technologies», vol. V, Dnipro, 26-28 April, 2017, pp. 125, 2017. [in Ukrainian]  G.M. Ashmarin, V.V. Aulin, M. Yu. Golubev,
S.D. Zvonkov, Grain Boundary Internal Friction of Unalloyed Copper Subjected to Continuous Laser Radiation, Physics and Chemistry of Materials Treatment, vol. 20, no. 5, pp. 476-478, 1986. [in Ukrainian]
 M.I. Chernovol, E.K. Solovykh, Prediction of Thickness of Solid-Lubricant Film Formed at Friction of Metal-Polymer Composite Coating, Journal of Friction and Wear, vol. 18, no. 2, pp. 40-45, 1997. [in Ukrainian]
 D. Vasilkov, I. Pustovoy, The Analysis of the Layer Formed by the Mineral Modifier of Surface of Friction, Мoscow: Trudy GOSNIITY, vol. 107, iss. 2, pp. 11-13. [in Russian]
 S. Baskar, G. Sriram, S. Arumugam, Experimental Analysis on Tribological Behaviour of Nano Based Bio-Lubricants Using Four Ball Tribometer, Tribology in Industry, vol. 37, no. 4, pp. 449-454, 2015.
 V. Aulin, A. Hrynkiv, S. Lysenko, I. Rohovskii, M. Chernovol, O. Lyashuk, T. Zamota, Studying Truck Transmission Oils Using the Method of Thermal-Oxidative Stability during Vehicle Operation,
Eastern-European Journal of Enterprise Technologies, vol. 1, no. 6(97), pp. 6-12, 2019, doi: 10.15587/1729-4061.2019.156150
 B. Basu, M. Kalin, Tribology of Ceramics and Composites: Materials Science Perspective, New York: Wiley, 2011.
 V. Aulin, T.N. Zamota, S. Lysenko, Increase of Machine Parts Performance Wear Resistance by Their Tribological Reconditioning and Control of Wear-In Processes, MOTROL. Commission of Motorization and Energetics in Agriculture, vol. 18, no. 2, pp. 89-96, 2016.
 V. Aulin, W. Arifa, S. Lysenko, A. Kuzyk,
Improving of the Wear Resistance of Working Parts Agricultural Machinery by the Implementation of the Effect of Self-Sharpening, International Journal of Engineering and Technology, vol. 5, no. 4, pp. 126-130, 2016,
 C. Anderberg, Z. Dimkovski, B.-G. Rosén, T.R. Thomas, Low Friction and Emission Cylinder Liner Surfaces and the Influence of Surface Topography and Scale, Tribology International, pp. 224-229, 2019, doi: 10.1016/j.triboint.2018.11.022
 T. Kuwahara, P.A. Romero, S. Makowski, V. Weihnacht, G. Moras, M. Moseler, Mechano-Chemical Decomposition of Organic Modifiers With Multiple Reactive Centres Induces Superlubricity of Ta-C, Nature Communications, vol. 10, no. 1, 151, 2019, doi: 10.1038/s41467-018-08042-8
 J. Yuansheng, L. Shenghua, Superlubricity of in Situ Generated Protective Layer on Worn Metal Surfaces in Presence of Mg6Si4O10(OH)8, in A. Erdemir, J.M. Martin (Ed.): Superlubricity. Elsevier, pp. 445-469, 2007, doi: 10.1016/B978-044452772-1/50055-X
 M. Ebrahimi, M.H. Shaeri, C. Gode, H. Armoon, M. Shamsborhan, The Synergistic Effect of Dilute Alloying and Nanostructuring of Copper on the Improvement of Mechanical and Tribological Response, Composites Part B: Engineering, vol.
164, pp. 508-516, 2019, doi:
 A. Dounaev, Friction Surfaces Modification Using Tribo-Compounds, World Applied Sciences Journal, vol. 31, no. 2, 272-276, 2014.
 A. Dykha, V. Aulin, O. Makovkin, S. Posonskiy,
Determining the Characteristics of Viscous Friction in the Sliding Supports Using the Method of Pendulum, EasternEuropean Journal of Enterprise Technologies, vol. 3, no. 7(87), pp. 4-10, 2017, doi: 10.15587/1729-4061.2017.99823
 D. Lutsak, P. Prysyazhnyuk, M. Burda, V. Aulin,
Development of a Method and an Apparatus for Tribotechnical Tests of Materials Under Loose Abrasive Friction, EasternEuropean Journal of Enterprise Technologies, vol. 5, no. 7(83), pp. 19-26, 2016, doi: 10.15587/1729-4061.2016.79913
 S. Kim, Y.J. Ahn, Y.H. Jang, Frictional Energy Dissipation for Coupled Systems Subjected to Harmonically Varying Loadsv Tribology International, vol. 134, pp. 205-210v 2019, doi: 10.1016/j.triboint.2019.01.021
 V. Aulin, V. Slon, S. Lysenko, D. Holub. Pat. 81598 Ukraine, The Work Piece Lubricating Composition, Declarant and Patent holders is the Kirovohrad National Technical University, №u201213907, declared 06.12.2012, published 10.07.2013, no. 13, 2013. [in Ukrainian]
 XADO Nanotechnology for Industrial, Oil for automotive diesel engines], available at
O%20M10G2k.pdf, accessed: 19.02.2019.
 C. Georgescu, L.C. Solea, L. Deleanu, The Influence of Degumming Process on Tribological Behaviour of Soybean Oil, Tribology in Industry, vol. 37, no. 3, pp. 330-335, 2015.
 E.T. Kang, Surface Modification of Fluoropolymers via Molecular Design. Advanced Materials, vol. 12, no. 20, pp. 1481-1494, 2000.  Z. Geng, D. Puhan, T. Reddyhoff, Using Acoustic